#------------------------------------------------------------------------------
#$Date: 2016-03-24 13:58:10 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179647 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/00/4510067.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4510067
loop_
_publ_author_name
'Lee, Jackson J.'
'Sobolev, Alexandre N.'
'Turner, Michael J.'
'Fuller, Rebecca O.'
'Iversen, Bo B.'
'Koutsantonis, George A.'
'Spackman, Mark A.'
_publ_section_title
;
 Molecular Imprisonment: Host Response to Guest Location, Orientation, and
 Dynamics in Clathrates of Dianin’s Compound
;
_journal_issue                   3
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              1296
_journal_paper_doi               10.1021/cg4018129
_journal_volume                  14
_journal_year                    2014
_chemical_formula_moiety         '6(C18 H20 O2), C6 H5 I'
_chemical_formula_sum            'C114 H125 I O12'
_chemical_formula_weight         1814.03
_chemical_name_systematic
;
 4-p-Hydroxyphenyl-2,2,4-trimethylchroman iodobenzene clathrate
;
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   26.971(1)
_cell_length_b                   26.971
_cell_length_c                   10.7851(3)
_cell_measurement_reflns_used    12270
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      30.44
_cell_measurement_theta_min      2.97
_cell_volume                     6794.4(3)
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
(compiled Nov  6 2009,16:24:50)
;
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
(compiled Nov  6 2009,16:24:50)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
(compiled Nov  6 2009,16:24:50)
;
_computing_molecular_graphics    'CrystalExplorer 3.2 (Wolff, et al., 2013'
_computing_publication_material  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS-2013 (Sheldrick, 2013)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 16.0009
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type
'Oxford Diffraction Xcalibur-S, Sapphire3 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'normal-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0948
_diffrn_reflns_av_unetI/netI     0.0505
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       38
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -38
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            29948
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.499
_diffrn_reflns_theta_min         2.982
_exptl_absorpt_coefficient_mu    0.420
_exptl_absorpt_correction_T_max  0.954
_exptl_absorpt_correction_T_min  0.937
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
(compiled Nov  6 2009,16:24:50)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.330
_exptl_crystal_description       prism
_exptl_crystal_F_000             2874
_exptl_crystal_size_max          0.240
_exptl_crystal_size_mid          0.180
_exptl_crystal_size_min          0.160
_refine_diff_density_max         1.020
_refine_diff_density_min         -0.565
_refine_diff_density_rms         0.080
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.163
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     199
_refine_ls_number_reflns         4591
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.162
_refine_ls_R_factor_all          0.1283
_refine_ls_R_factor_gt           0.1143
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0200P)²+70.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2206
_refine_ls_wR_factor_ref         0.2268
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3841
_reflns_number_total             4591
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cg4018129_si_002.cif
_cod_data_source_block           973707
_cod_original_cell_volume        6794.4(5)
_cod_database_code               4510067
#BEGIN Tags that were not found in dictionaries:
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.906
_shelx_estimated_absorpt_t_max   0.936
_shelxl_version_number           2013-4
#END Tags that were not found in dictionaries
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.06288(12) 0.11795(12) 0.4809(2) 0.0290(6) Uani 1 1 d . . . . .
H1 H 0.0809 0.0996 0.4847 0.043 Uiso 1 1 calc R U . . .
O2 O 0.08839(12) 0.26415(14) -0.1313(2) 0.0346(7) Uani 1 1 d . . . . .
C1 C 0.11071(16) 0.2268(2) -0.0957(3) 0.0318(8) Uani 1 1 d . . . . .
C2 C 0.08845(15) 0.29995(19) -0.0414(3) 0.0286(8) Uani 1 1 d . . . . .
C3 C 0.12026(15) 0.31407(17) 0.0680(3) 0.0260(7) Uani 1 1 d . . . . .
C4 C 0.15824(15) 0.28824(18) 0.0984(3) 0.0275(7) Uani 1 1 d . . . . .
C5 C 0.16536(16) 0.26107(19) -0.0212(3) 0.0302(8) Uani 1 1 d . . . . .
H5A H 0.1942 0.2919 -0.0745 0.036 Uiso 1 1 calc R U . . .
H5B H 0.1806 0.2356 0.0013 0.036 Uiso 1 1 calc R U . . .
C6 C 0.21854(16) 0.33620(19) 0.1349(3) 0.0319(8) Uani 1 1 d . . . . .
H6A H 0.2162 0.3550 0.2106 0.048 Uiso 1 1 calc R U . . .
H6B H 0.2345 0.3644 0.0677 0.048 Uiso 1 1 calc R U . . .
H6C H 0.2433 0.3198 0.1495 0.048 Uiso 1 1 calc R U . . .
C7 C 0.11746(16) 0.35320(17) 0.1471(3) 0.0284(8) Uani 1 1 d . . . . .
H7 H 0.1392 0.3635 0.2216 0.034 Uiso 1 1 calc R U . . .
C8 C 0.08432(17) 0.37768(18) 0.1215(3) 0.0308(8) Uani 1 1 d . . . . .
H8 H 0.0833 0.4044 0.1773 0.037 Uiso 1 1 calc R U . . .
C9 C 0.05224(16) 0.36264(18) 0.0123(4) 0.0310(8) Uani 1 1 d . . . . .
H9 H 0.0288 0.3788 -0.0058 0.037 Uiso 1 1 calc R U . . .
C10 C 0.05437(15) 0.32464(18) -0.0688(3) 0.0294(8) Uani 1 1 d . . . . .
H10 H 0.0329 0.3149 -0.1436 0.035 Uiso 1 1 calc R U . . .
C11 C 0.13302(15) 0.24436(17) 0.2045(3) 0.0250(7) Uani 1 1 d . . . . .
C12 C 0.16178(16) 0.21595(18) 0.2454(3) 0.0287(8) Uani 1 1 d . . . . .
H12 H 0.1975 0.2254 0.2086 0.034 Uiso 1 1 calc R U . . .
C13 C 0.13980(16) 0.17473(17) 0.3372(3) 0.0276(7) Uani 1 1 d . . . . .
H13 H 0.1603 0.1564 0.3629 0.033 Uiso 1 1 calc R U . . .
C14 C 0.08748(15) 0.16014(16) 0.3919(3) 0.0234(7) Uani 1 1 d . . . . .
C15 C 0.05893(15) 0.18840(17) 0.3562(3) 0.0243(7) Uani 1 1 d . . . . .
H15 H 0.0238 0.1795 0.3951 0.029 Uiso 1 1 calc R U . . .
C16 C 0.08141(15) 0.22980(17) 0.2635(3) 0.0248(7) Uani 1 1 d . . . . .
H16 H 0.0611 0.2486 0.2396 0.030 Uiso 1 1 calc R U . . .
C17 C 0.12512(18) 0.2087(2) -0.2184(3) 0.0361(9) Uani 1 1 d . . . . .
H17A H 0.1558 0.2424 -0.2601 0.054 Uiso 1 1 calc R U . . .
H17B H 0.0910 0.1911 -0.2713 0.054 Uiso 1 1 calc R U . . .
H17C H 0.1378 0.1810 -0.2024 0.054 Uiso 1 1 calc R U . . .
C18 C 0.06305(18) 0.1751(2) -0.0292(4) 0.0392(10) Uani 1 1 d . . . . .
H18A H 0.0298 0.1556 -0.0843 0.059 Uiso 1 1 calc R U . . .
H18B H 0.0521 0.1878 0.0458 0.059 Uiso 1 1 calc R U . . .
H18C H 0.0765 0.1487 -0.0064 0.059 Uiso 1 1 calc R U . . .
C01 C 0.0130(3) 0.0033(3) 0.0123(12) 0.0330(19) Uiso 0.1667 1 d G . P A -1
C02 C -0.0367(5) 0.0002(7) 0.0545(11) 0.0330(19) Uiso 0.1667 1 d DG . P A -1
H02 H -0.0642 -0.0013 -0.0029 0.040 Uiso 0.1667 1 calc R U P A -1
C03 C -0.0466(7) -0.0007(9) 0.1796(10) 0.0330(19) Uiso 0.1667 1 d G . P A -1
H03 H -0.0809 -0.0028 0.2088 0.040 Uiso 0.1667 1 calc R U P A -1
C04 C -0.0068(6) 0.0015(7) 0.2624(11) 0.0330(19) Uiso 0.1667 1 d G . P A -1
H04 H -0.0136 0.0009 0.3490 0.040 Uiso 0.1667 1 calc R U P A -1
C05 C 0.0430(6) 0.0046(8) 0.2202(10) 0.0330(19) Uiso 0.1667 1 d G . P A -1
H05 H 0.0704 0.0062 0.2777 0.040 Uiso 0.1667 1 calc R U P A -1
C06 C 0.0529(5) 0.0056(7) 0.0951(9) 0.0330(19) Uiso 0.1667 1 d DG . P A -1
H06 H 0.0871 0.0077 0.0659 0.040 Uiso 0.1667 1 calc R U P A -1
I1 I 0.02791(9) 0.00475(10) -0.17975(16) 0.0478(5) Uani 0.1667 1 d D . P A -1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
C14 O1 H1 109.5
C2 O2 C1 116.5(3)
O2 C1 C5 109.1(4)
O2 C1 C18 107.7(3)
C5 C1 C18 115.2(3)
O2 C1 C17 104.6(3)
C5 C1 C17 109.2(3)
C18 C1 C17 110.4(4)
O2 C2 C3 125.1(3)
O2 C2 C10 114.5(3)
C3 C2 C10 120.4(4)
C7 C3 C2 117.9(3)
C7 C3 C4 121.0(3)
C2 C3 C4 121.1(3)
C3 C4 C11 111.7(3)
C3 C4 C6 109.7(3)
C11 C4 C6 109.3(3)
C3 C4 C5 107.9(3)
C11 C4 C5 111.6(3)
C6 C4 C5 106.4(3)
C1 C5 C4 114.7(3)
C1 C5 H5A 108.6
C4 C5 H5A 108.6
C1 C5 H5B 108.6
C4 C5 H5B 108.6
H5A C5 H5B 107.6
C4 C6 H6A 109.5
C4 C6 H6B 109.5
H6A C6 H6B 109.5
C4 C6 H6C 109.5
H6A C6 H6C 109.5
H6B C6 H6C 109.5
C8 C7 C3 122.3(3)
C8 C7 H7 118.8
C3 C7 H7 118.8
C7 C8 C9 119.1(4)
C7 C8 H8 120.5
C9 C8 H8 120.5
C10 C9 C8 120.3(3)
C10 C9 H9 119.9
C8 C9 H9 119.9
C9 C10 C2 120.0(3)
C9 C10 H10 120.0
C2 C10 H10 120.0
C16 C11 C12 116.6(3)
C16 C11 C4 123.4(3)
C12 C11 C4 120.0(3)
C13 C12 C11 122.1(3)
C13 C12 H12 119.0
C11 C12 H12 119.0
C12 C13 C14 119.9(3)
C12 C13 H13 120.1
C14 C13 H13 120.1
O1 C14 C15 118.6(3)
O1 C14 C13 122.0(3)
C15 C14 C13 119.4(3)
C14 C15 C16 120.2(3)
C14 C15 H15 119.9
C16 C15 H15 119.9
C15 C16 C11 121.7(3)
C15 C16 H16 119.1
C11 C16 H16 119.1
C1 C17 H17A 109.5
C1 C17 H17B 109.5
H17A C17 H17B 109.5
C1 C17 H17C 109.5
H17A C17 H17C 109.5
H17B C17 H17C 109.5
C1 C18 H18A 109.5
C1 C18 H18B 109.5
H18A C18 H18B 109.5
C1 C18 H18C 109.5
H18A C18 H18C 109.5
H18B C18 H18C 109.5
C06 C01 C02 120.2
C06 C01 I1 120.0
C02 C01 I1 119.8
C03 C02 C01 120.0
C03 C02 H02 120.0
C01 C02 H02 120.0
C02 C03 C04 119.8
C02 C03 H03 120.1
C04 C03 H03 120.1
C03 C04 C05 120.2
C03 C04 H04 119.9
C05 C04 H04 119.9
C06 C05 C04 120.0
C06 C05 H05 120.0
C04 C05 H05 120.0
C05 C06 C01 119.7
C05 C06 H06 120.1
C01 C06 H06 120.1
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
O1 C14 1.379(4)
O1 H1 0.8500
O2 C2 1.367(5)
O2 C1 1.461(5)
C1 C5 1.520(5)
C1 C18 1.522(6)
C1 C17 1.526(5)
C2 C3 1.395(5)
C2 C10 1.410(5)
C3 C7 1.388(5)
C3 C4 1.535(5)
C4 C11 1.539(5)
C4 C6 1.539(5)
C4 C5 1.542(5)
C5 H5A 0.9900
C5 H5B 0.9900
C6 H6A 0.9800
C6 H6B 0.9800
C6 H6C 0.9800
C7 C8 1.379(5)
C7 H7 0.9500
C8 C9 1.396(5)
C8 H8 0.9500
C9 C10 1.371(6)
C9 H9 0.9500
C10 H10 0.9500
C11 C16 1.396(5)
C11 C12 1.406(5)
C12 C13 1.382(5)
C12 H12 0.9500
C13 C14 1.393(5)
C13 H13 0.9500
C14 C15 1.382(5)
C15 C16 1.392(5)
C15 H15 0.9500
C16 H16 0.9500
C17 H17A 0.9800
C17 H17B 0.9800
C17 H17C 0.9800
C18 H18A 0.9800
C18 H18B 0.9800
C18 H18C 0.9800
C01 C06 1.376(9)
C01 C02 1.380(9)
C01 I1 2.107(14)
C02 C03 1.373(9)
C02 H02 0.9500
C03 C04 1.376(9)
C03 H03 0.9500
C04 C05 1.379(9)
C04 H04 0.9500
C05 C06 1.373(9)
C05 H05 0.9500
C06 H06 0.9500
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O1 H1 O1 0.85 1.94 2.787(3) 171.3 11_556
